LMucko/crystallography-open-database huggingface dataset:
The crystal structure of monoclinic langbanite: (Mn,Ca,Fe,Mg)2+4(Mn,Fe)3+9Sb5+[O16(SiO4)2]
Giuseppetti, G.; Mazzi, F.; Tadini, C.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 193–211; doi:

data_9009368
_publ_section_title
;
 The crystal structure of monoclinic langbanite:
 (Mn,Ca,Fe,Mg)2+4(Mn,Fe)3+9Sb5+[O16(SiO4)2]
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              193
_journal_page_last               211
_journal_volume                  1991
_journal_year                    1991
_chemical_compound_source        'Langban, Sweden'
_chemical_formula_sum            'Ca0.79 Fe6.09 Mg0.14 Mn31.98 O72 Sb3 Si6'
_chemical_name_mineral           Langbanite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.03
_cell_angle_gamma                90
_cell_length_a                   11.561
_cell_length_b                   20.05
_cell_length_c                   11.075
_cell_formula_units_Z            2
_cell_volume                     2567.163
_database_code_amcsd             0014850
_exptl_crystal_density_diffrn    4.939
_cod_original_formula_sum        'Sb3 Mn31.98 Ca.79 Mg.14 Fe6.09 Si6 O72'
_cod_database_code               9009368
The crystal structures of kieserite-type compounds. I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
Wildner, M.; Giester, G.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 296–306; doi:

data_9009369
_publ_section_title
;
 The crystal structures of kieserite-type compounds.
 I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              296
_journal_page_last               306
_journal_volume                  1991
_journal_year                    1991
_chemical_compound_source        Synthetic
_chemical_formula_sum            'H2 Mn O5 S'
_chemical_name_mineral           Szmikite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 118.11
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.116
_cell_length_b                   7.667
_cell_length_c                   7.920
_cell_volume                     381.134
_database_code_amcsd             0014851
_exptl_crystal_density_diffrn    2.946
_cod_depositor_comments
;
     Z value introduced to be consistent with given formula
                                      miguel
;
_cod_original_formula_sum        'Mn S O5 H2'
_cod_database_code               9009369
The crystal structures of kieserite-type compounds. I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
Wildner, M.; Giester, G.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 296–306; doi:

data_9009370
_publ_section_title
;
 The crystal structures of kieserite-type compounds.
 I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              296
_journal_page_last               306
_journal_volume                  1991
_journal_year                    1991
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe H2 O5 S'
_chemical_name_mineral           Szomolnokite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 118.65
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.078
_cell_length_b                   7.549
_cell_length_c                   7.773
_cell_volume                     364.475
_database_code_amcsd             0014852
_exptl_crystal_density_diffrn    3.097
_cod_depositor_comments
;
     Z value introduced to be consistent with given formula
                                      miguel
;
_cod_original_formula_sum        'Fe S O5 H2'
_cod_database_code               9009370
The crystal structures of kieserite-type compounds. I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
Wildner, M.; Giester, G.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 296–306; doi:

data_9009371
_publ_section_title
;
 The crystal structures of kieserite-type compounds.
 I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              296
_journal_page_last               306
_journal_volume                  1991
_journal_year                    1991
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Co H2 O5 S'
_chemical_name_mineral           Cobaltkieserite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 118.56
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.960
_cell_length_b                   7.586
_cell_length_c                   7.621
_cell_volume                     353.415
_database_code_amcsd             0014853
_exptl_crystal_density_diffrn    3.252
_cod_depositor_comments
;
     Z value introduced to be consistent with given formula
                                      miguel
;
_cod_original_formula_sum        'Co S O5 H2'
_cod_database_code               9009371
The crystal structures of kieserite-type compounds. I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
Wildner, M.; Giester, G.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 296–306; doi:

data_9009372
_publ_section_title
;
 The crystal structures of kieserite-type compounds.
 I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              296
_journal_page_last               306
_journal_volume                  1991
_journal_year                    1991
_chemical_compound_source        Synthetic
_chemical_formula_sum            'H2 Ni O5 S'
_chemical_name_mineral           Dwornikite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 117.79
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.824
_cell_length_b                   7.594
_cell_length_c                   7.457
_cell_volume                     341.862
_database_code_amcsd             0014854
_exptl_crystal_density_diffrn    3.357
_cod_depositor_comments
;
     Z value introduced to be consistent with given formula
                                      miguel
;
_cod_original_formula_sum        'Ni S O5 H2'
_cod_database_code               9009372
The crystal structures of kieserite-type compounds. I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
Wildner, M.; Giester, G.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 296–306; doi:

data_9009373
_publ_section_title
;
 The crystal structures of kieserite-type compounds.
 I. Crystal structures of Me(II)SO4*H2O (Me = Mn,Fe,Co,Ni,Zn)
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              296
_journal_page_last               306
_journal_volume                  1991
_journal_year                    1991
_chemical_compound_source        Synthetic
_chemical_formula_sum            'H2 O5 S Zn'
_chemical_name_mineral           Gunningite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 118.19
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.925
_cell_length_b                   7.591
_cell_length_c                   7.635
_cell_volume                     353.748
_database_code_amcsd             0014855
_exptl_crystal_density_diffrn    3.370
_cod_depositor_comments
;
     Z value introduced to be consistent with given formula
                                      miguel
;
_cod_original_formula_sum        'Zn S O5 H2'
_cod_database_code               9009373
The revised crystal structure of roggianite: Ca2[Be(OH)2Al2Si4O13]<2.5H2O
Giuseppetti, G.; Mazzi, F.; Tadini, C.; Galli, E.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 307–314; doi:

data_9009374
_publ_section_title
;
 The revised crystal structure of roggianite: Ca2[Be(OH)2Al2Si4O13]<2.5H2O
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              307
_journal_page_last               314
_journal_volume                  1991
_journal_year                    1991
_chemical_compound_source        'Val Vigezzo, Novara, Italy'
_chemical_formula_sum            'Al2 Be Ca2 H7.56 O17.34 Si4'
_chemical_name_mineral           Roggianite
_space_group_IT_number           140
_symmetry_space_group_name_Hall  '-I 4 2c'
_symmetry_space_group_name_H-M   'I 4/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   18.33
_cell_length_b                   18.33
_cell_length_c                   9.16
_cell_volume                     3077.658
_database_code_amcsd             0014856
_exptl_crystal_density_diffrn    2.333
_cod_original_formula_sum        'Ca2 Be O17.34 H7.56 Al2 Si4'
_cod_database_code               9009374
Cation substitution in the apatite tetrahedral site: crystal structures of type hydroxylellestadtite and type fermorite Locality: Crestmore, California, USA
Hughes, J. M.; Drexler, J. W.; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 327–336; doi:

data_9009375
_publ_section_title
;
 Cation substitution in the apatite tetrahedral site:
 crystal structures of type hydroxylellestadtite and type fermorite
 Locality: Crestmore, California, USA
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              327
_journal_page_last               336
_journal_volume                  1991
_journal_year                    1991
_chemical_formula_sum            'Ca5 Cl0.24 F0.08 H0.68 O12.68 S1.5 Si1.5'
_chemical_name_mineral           Hydroxylellestadite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2c'
_symmetry_space_group_name_H-M   'P 1 1 21/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                119.9483
_cell_formula_units_Z            2
_cell_length_a                   9.5224
_cell_length_b                   9.5268
_cell_length_c                   6.9087
_cell_volume                     543.058
_exptl_crystal_density_diffrn    3.083
_cod_original_formula_sum        'Ca5 (Si1.5 S1.5) O12.68 F.08 Cl.24 H.68'
_cod_database_code               9009375
Cation substitution in the apatite tetrahedral site: crystal structures of type hydroxylellestadtite and type fermorite Locality: Sitipar deposit, India
Hughes J M; Drexler J W; Neues Jahrbuch fur Mineralogie, Monatshefte 1991 (1991) 327–336; doi:

data_9009376
_publ_section_title
;
 Cation substitution in the apatite tetrahedral site:
 crystal structures of type hydroxylellestadtite and type fermorite
 Locality: Sitipar deposit, India
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              327
_journal_page_last               336
_journal_volume                  1991
_journal_year                    1991
_chemical_formula_sum            'As1.5 Ca4.2 F0.345 H0.02 O12.654 P1.5 Sr0.8'
_chemical_name_mineral           Fermorite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2c'
_symmetry_space_group_name_H-M   'P 1 1 21/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                119.971
_cell_formula_units_Z            2
_cell_length_a                   9.5935
_cell_length_b                   9.5966
_cell_length_c                   6.9754
_cell_volume                     556.315
_cod_original_formula_sum        '(Ca4.2 Sr.8) (As1.5 P1.5) O12.654 F.345 H.02'
_cod_database_code               9009376
The crystal structure of pseudoboleite: Pb31Cu24Cl62(OH)48; its relations with the structures of boleite and cumengeite
Giuseppetti, G.; Mazzi, F.; Tadini, C.; Neues Jahrbuch fur Mineralogie, Monatshefte 1992 (1992) 113–126; doi:

data_9009377
_publ_section_title
;
 The crystal structure of pseudoboleite: Pb31Cu24Cl62(OH)48;
 its relations with the structures of boleite and cumengeite
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              113
_journal_page_last               126
_journal_volume                  1992
_journal_year                    1992
_chemical_compound_source        'Boleo, Baja California, Mexico'
_chemical_formula_sum            'Cl31 Cu12 H24 O24 Pb15.5'
_chemical_name_mineral           Pseudoboleite
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   15.24
_cell_length_b                   15.24
_cell_length_c                   30.74
_cell_volume                     7139.599
_database_code_amcsd             0014859
_exptl_crystal_density_diffrn    5.099
_cod_original_formula_sum        'Pb15.5 Cu12 Cl31 (O24 H24)'
_cod_database_code               9009377
On beaverite: new occurrence, chemical data and crystal structure Locality: Grand Reef mine, Graham County, Arizona, USA
Breidenstein, B.; Schluter, J.; Gebhard, G.; Neues Jahrbuch fur Mineralogie, Monatshefte 1992 (1992) 213–220; doi:

data_9009378
_publ_section_title
;
 On beaverite: new occurrence, chemical data and crystal structure
 Locality: Grand Reef mine, Graham County, Arizona, USA
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              213
_journal_page_last               220
_journal_volume                  1992
_journal_year                    1992
_chemical_formula_sum            'Fe3 H6 O14 Pb S2'
_chemical_name_mineral           Beaverite
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   7.205
_cell_length_b                   7.205
_cell_length_c                   16.994
_cell_volume                     764.002
_exptl_crystal_density_diffrn    4.362
_cod_data_source_file            cifdata.txt
_cod_data_source_block           'global_11487'
_cod_original_cell_volume        764.001
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_original_formula_sum        'Pb Fe3 S2 O14 H6'
_cod_database_code               9009378
_database_code_amcsd 0014860
Crystal structures of synthetic Na-REE-Si oxyapatites, synthetic monoclinic britholite Locality: synthetic
Hughes, J. M.; Mariano, A. N.; Drexler, J. W.; Neues Jahrbuch fur Mineralogie, Monatshefte 1992 (1992) 311–319; doi:

data_9009379
_publ_section_title
;Crystal structures of synthetic Na-REE-Si oxyapatites, synthetic monoclinic
 britholite Locality: synthetic
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              311
_journal_page_last               319
_journal_volume                  1992
_journal_year                    1992
_chemical_compound_source        Synthetic
_chemical_formula_sum            'F0.45 La4.277 Na0.723 O12.55 Si3'
_chemical_name_mineral           Britholite-(La)
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2c'
_symmetry_space_group_name_H-M   'P 1 1 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120.04
_cell_length_a                   9.678
_cell_length_b                   9.682
_cell_length_c                   7.1631
_cell_formula_units_Z            2
_cell_volume                     581.041
_database_code_amcsd             0014862
_exptl_crystal_density_diffrn    5.169
_cod_original_cell_volume        581.042
_cod_original_formula_sum        '(La4.277 Na.723) Si3 O12.55 F.45'
_cod_database_code               9009379
Crystal structures of synthetic Na-REE-Si oxyapatites, synthetic monoclinic britholite Locality: synthetic
Hughes, J. M.; Mariano, A. N.; Drexler, J. W.; Neues Jahrbuch fur Mineralogie, Monatshefte 1992 (1992) 311–319; doi:

data_9009380
_publ_section_title
;Crystal structures of synthetic Na-REE-Si oxyapatites, synthetic monoclinic
 britholite Locality: synthetic
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              311
_journal_page_last               319
_journal_volume                  1992
_journal_year                    1992
_chemical_compound_source        Synthetic
_chemical_formula_sum            'F0.19 Gd4.405 Na0.595 O12.81 Si3'
_chemical_name_mineral           Britholite-(Gd)
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2c'
_symmetry_space_group_name_H-M   'P 1 1 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120.01
_cell_length_a                   9.410
_cell_length_b                   9.413
_cell_length_c                   6.8740
_cell_formula_units_Z            2
_cell_volume                     527.247
_database_code_amcsd             0014863
_exptl_crystal_density_diffrn    6.294
_cod_original_formula_sum        '(Gd4.405 Na.595) Si3 O12.81 F.19'
_cod_database_code               9009380
Structural study of a magnesian ferrocarpholite: Are carpholites monoclinic?
Ferraris, G.; Ivaldi, G.; Goffe, B.; Neues Jahrbuch fur Mineralogie, Monatshefte 1992 (1992) 337–347; doi:

data_9009381
_publ_section_title
;
 Structural study of a magnesian ferrocarpholite: Are carpholites monoclinic?
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              337
_journal_page_last               347
_journal_volume                  1992
_journal_year                    1992
_chemical_compound_source        'Mascate nappes, Ruwi, Oman'
_chemical_formula_sum            'Al2 Fe0.76 H4 Mg0.24 O10 Si2'
_chemical_name_mineral           Ferrocarpholite
_space_group_IT_number           68
_symmetry_space_group_name_Hall  '-C 2a 2ac'
_symmetry_space_group_name_H-M   'C c c a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   13.797
_cell_length_b                   20.20
_cell_length_c                   5.116
_cell_volume                     1425.826
_database_code_amcsd             0014864
_exptl_crystal_density_diffrn    3.004
_cod_original_sg_symbol_H-M      'C c c a'
_cod_original_formula_sum        '(Fe.76 Mg.24) Al2 Si2 O10 H4'
_cod_database_code               9009381
The crystal structure of vikingite
Makovicky, E.; Mumme, W. G.; Madsen, I. C.; Neues Jahrbuch fur Mineralogie, Monatshefte 1992 (1992) 454–468; doi:

data_9009382
_publ_section_title
;
 The crystal structure of vikingite
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              454
_journal_page_last               468
_journal_volume                  1992
_journal_year                    1992
_chemical_compound_source        'La Roche Balue, France'
_chemical_formula_sum            'Ag1.78 Bi5.78 Pb5.44 S15'
_chemical_name_mineral           Vikingite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.59
_cell_angle_gamma                90
_cell_length_a                   13.598
_cell_length_b                   4.112
_cell_length_c                   25.2490
_cell_formula_units_Z            2
_cell_volume                     1405.083
_database_code_amcsd             0014865
_exptl_crystal_density_diffrn    7.110
_cod_original_formula_sum        'Bi5.78 Ag1.78 Pb5.44 S15'
_cod_database_code               9009382
Huanghoite-(Ce), BaCe(CO3)2F, from Khibina, Kola peninsula, Russia: Redetermination of the crystal structure with a discussion on space group symmetry Locality: Khibina, Kola Peninsula, Russia
Yang, Z. M.; Pertlik, F.; Neues Jahrbuch fur Mineralogie, Monatshefte 1993 (1993) 163–171; doi:

data_9009383
_publ_section_title
;Huanghoite-(Ce), BaCe(CO3)2F, from Khibina, Kola peninsula, Russia:
 Redetermination of the crystal structure with a discussion on space group
 symmetry Locality: Khibina, Kola Peninsula, Russia
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              163
_journal_page_last               171
_journal_volume                  1993
_journal_year                    1993
_chemical_compound_source        'Khibina, Kola Peninsula, Russia'
_chemical_formula_sum            'C2 Ba Ce F O6'
_chemical_name_mineral           Huanghoite-(Ce)
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   5.072
_cell_length_b                   5.072
_cell_length_c                   38.46
_cell_formula_units_Z            6
_cell_volume                     856.837
_database_code_amcsd             0014866
_exptl_crystal_density_diffrn    4.843
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_original_formula_sum        'Ba Ce C2 O6 F'
_cod_database_code               9009383
The crystal structure of nealite: Pb4Fe(AsO3)2Cl4*2H2O
Giuseppetti, G.; Mazzi, F.; Tadini, C.; Neues Jahrbuch fur Mineralogie, Monatshefte 1993 (1993) 278–288; doi:

data_9009384
_publ_section_title
;
 The crystal structure of nealite: Pb4Fe(AsO3)2Cl4*2H2O
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Monatshefte'
_journal_page_first              278
_journal_page_last               288
_journal_volume                  1993
_journal_year                    1993
_chemical_compound_source        'Laurion, Greece'
_chemical_formula_sum            'As2 Cl4 Fe H4 O8 Pb4'
_chemical_name_mineral           Nealite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                96.4
_cell_angle_beta                 89.5
_cell_angle_gamma                97.8
_cell_formula_units_Z            1
_cell_length_a                   6.53
_cell_length_b                   10.23
_cell_length_c                   5.588
_cell_volume                     367.523
_database_code_amcsd             0014867
_exptl_crystal_density_diffrn    5.911
_cod_original_formula_sum        'Pb4 Fe As2 O8 Cl4 H4'
_cod_database_code               9009384